# Giant Rashba effect at the topological surface of PrGe revealing antiferromagnetic spintronics

## Abstract

Rashba spin-orbit splitting in the magnetic materials opens up a new perspective in the field of spintronics. Here, we report a giant Rashba spin-orbit splitting on the PrGe [010] surface in the paramagnetic phase with Rashba coefficient α R  = 5 eVÅ. We find that α R can be tuned in this system as a function of temperature at different magnetic phases. Rashba type spin polarized surface states originates due to the strong hybridization between Pr 4f states with the conduction electrons. Significant changes observed in the spin polarized surface states across the magnetic transitions are due to the competition between Dzyaloshinsky-Moriya interaction and exchange interaction present in this system. Presence of Dzyaloshinsky-Moriya interaction on the topological surface give rise to Saddle point singularity which leads to electron-like and hole-like Rashba spin split bands in the $$\bar{{\boldsymbol{Z}}}^{\prime} -\bar{{\boldsymbol{\Gamma }}}-\bar{{\boldsymbol{Z}}}$$ and $$\bar{{\boldsymbol{X}}}^{\prime} -\bar{{\boldsymbol{\Gamma }}}-\bar{{\boldsymbol{X}}}$$ directions, respectively. Supporting evidences of Dzyaloshinsky-Moriya interaction have been obtained as anisotropic magnetoresistance with respect to field direction and first-order type hysteresis in the X-ray diffraction measurements. A giant negative magnetoresistance of 43% in the antiferromagnetic phase and tunable Rashba parameter with temperature makes this material a suitable candidate for application in the antiferromagnetic spintronic devices.

## Introduction

One of the main challenges in the field of spintronics is to manipulate the spin structures by electric and spin currents. In this context the materials with Rashba spin-orbit (SO) coupling1 have gained a huge amount of interest due to their use in the Spintronics technology2, 3. Rashba effect in the non-magnetic systems has been extensively studied4,5,6,7 but there are very few reports on the magnetic metallic systems showing the Rashba effect8,9,10. In ferromagnetic (FM) materials with the SO splitting the magnetization reversal gives rise to Rashba effect which can be used for the giant magnetoresistance devices and spin transfer torque device applications9, 10. Antiferromagnetic (AFM) materials are the hidden magnets and the magnetism in these systems is difficult to probe experimentally. The magnetization reversal in the AFM systems will not make any change because of zero net magnetic moment. In such a case, the rotation of the spins will lead to the change in the resistance and has important technological applications11, 12. The anisotropic magnetoresistance in these AFM systems is linked to the SO interaction. Hence, the AFM systems which have significant anisotropy can be the promising candidates for the AFM spintronic devices13.

In recent years there has been flurry of research in understanding the anisotropic magnetic properties of several Pr-based compounds14,15,16,17,18. Pr-based compounds exhibit a variety of ground state properties due to the critical role of crystalline-electric-field effects, quadrupolar fluctuations etc.14,15,16,17,18. The mechanism of the heavy Fermion behavior in Pr-compounds is quite different from the usual Kondo route to heavy Fermions in Ce-based compounds. The crystal structural, transport and magnetic properties of PrGe single crystal have been studied in great detail19,20,21. PrGe crystallizes in CrB type crystal structure with Cmcm space group (Fig. 1(a))19. Magnetic studies on PrGe single crystal showed two magnetic transitions at 44 K and 41.5 K related to the AFM and FM transitions respectively19. Interestingly, a higher effective magnetic moment of Pr in PrGe has been observed for [010] crystallographic orientation ~3.90 μ B , which is not only higher than the effective moment of free Pr3+ ion ~3.58 μ B but also higher than the moment observed along [100] (~3.78 μ B ) and [001] (~3.71 μ B ) crystallographic orientations. Since, the effective magnetic moment is related to the magnetocrystalline anisotropy (MCA), which is intrinsically linked to the SO interaction. Hence, to understand the origin of different magnetic ground states in PrGe it is utmost important to investigate the nature of SO interaction present in this system.

In the present work, we have investigated the band structure and electronic density of states by angle resolved photoemission (ARPES) and resonant photoemission measurements, respectively. We report that the Rashba type SO splitting observed on the topological surface of PrGe [010] single crystal is due to the fact that the system behaves like a weak ferromagnetic system which is associated with the spin-canting antiferromagnetic coupling between the Pr atoms. The magnetism is due to the indirect exchange interaction between the localized moment carried by the Pr 4f electrons which induces a spin-polarization in the conduction electrons and give rise to Rashba type spin split bands. There is a competition between Dzyaloshinsky-Moriya (DM) interaction22 and exchange interaction which actually changes the spin-polarization of the conduction electrons and give rise to different magnetic phases in PrGe.

## Results and Discussions

High resolution ARPES measurements have been performed to determine the electronic band structure of PrGe [010] single crystal at  = 28 eV. The surface 2D Brillouin zone which has been probed is shown in Fig. 1(a). In Fig. 1(b,c) we have shown the band structure in the paramagnetic (PM) phase at 100 K and FM phase at 20 K, respectively. The most interesting observation in the band structure is that a flat band at −0.12 eV shows a Rashba type SO splitting in the PM and FM phase (Fig. 1(b,c)) near the Γ point. The spin split bands have hole-like character. The presence of Rashba SO splitting indicates that there is symmetry breaking at the surface which leads to spin-polarized surface states. We find that the spin polarized surface states which lies between −0.5 eV to E F gets modified across the magnetic transition (Fig. 1(b,c)). A non-dispersive flat band at −0.12 eV emerges either due to the singular density of states within the dislocations23 or due to the interaction between electrons or holes on the surface of materials because of nontrivial topology of the electronic spectrum in bulk. In the gapless topological systems, it is reported that the bulk-surface and bulk-vortex correspondence produces such flat bands on the surface of the system or in the core of topological defects23,24,25. We find that the Rashba effect observed in this magnetic system is quite different from the Rashba effect reported for the other magnetic systems like Gd, Tb etc.8, 9, hence its origin need to be explored.

To understand the role of surface states and its correlation with the magnetism present in this system, we have performed a detailed band structure study as a function of temperature as shown in Fig. 1(d–m). The behavior of the split bands in the PM phase remains similar (Fig. 1(d–h)) between 100 K to 60 K. A drastic change is observed in the bands at and below 51 K (Fig. 1(i)) which is close to the AFM transition. In the AFM phase, the spin split feature in the hole-like bands disappears and is found to be overlapped with the electron-like bands. On further lowering the temperature, in the FM phase, we have observed both the overlapped electron-like and hole-like bands with prominent spin split features (Fig. 1(k–m)). The changes in the band structure across the magnetic transition is due to the mixing of the Pr 4f states with the other valence states in this system which actually causes a change in the spin polarization of the conduction electrons. Similar kind of changes in the band structure have been observed in CeSb across the PM to AFM phase transition26 which was attributed to the mixing of Sb 5p bands with the Ce 4f  bands.

We find that the Rashba type SO splitting is large in the PM phase. Hence, to understand the character of the bands which give rise to the splitting, we have performed the resonant photoemission (RPES) measurements at room temperature. RPES has been performed across the Pr 4d–4f resonance in the photon energy range from 110 to 140 eV. The RPES data are plotted in the contour plot as shown in Fig. 2(a), where 4 prominent features marked as A, B, C and D at −0.65, −3.2, −5 and −8 eV respectively, are observed. Across the Pr 4d to 4f resonance, feature A shows a significant enhancement in intensity (Fig. 2(a)). The constant initial state (CIS) spectrum for the feature A at −0.65 eV has been plotted in the inset of Fig. 2(a) using the standard method discussed elsewhere27, 28. To understand the character of this feature Fano line profile29 of the form $$\sigma (h\nu )={\sigma }_{a}\frac{{(q+\varepsilon )}^{2}}{1+{\varepsilon }^{2}}+{\sigma }_{b}$$ and ε = ( − E 0)/W has been fitted and shown in the inset of Fig. 2(a) with a solid line. Here, the parameters E 0, q and W represents the resonance energy, discrete/continuum mixing strength and the half-width of the line, respectively. The value of the parameters determined from fitting are E 0 = 125 ± 0.02 eV, q = 3.69 ± 0.01 and W = 1.92 ± 0.01 eV. The larger value of q indicates that the states at −0.65 eV BE (feature A) is localized in nature. Two broad features B and C do not show the resonance. We find that the Pr 4d–4f resonance in PrGe is quite different from the results reported for thick Pr films30. The localized Pr 4f states at −3.6 eV in bulk Pr films show a larger enhancement than the features near E F which are mainly the Pr 5d states30. However, in PrGe the enhancement of the states near E F gives a clear indication that both the localized and the itinerant character of the Pr 4f states play important role in the magnetism of this system. Similar enhancement of Pr 4f states near E F has been observed in the RPES spectra of high T C superconductor Y1−x Pr x Ba2Cu3O7−δ 31 which has been attributed to the hybridization of the Pr 4f states with the Cu 3d and O 2p states in this system. For PrGe, the resonance has been observed at ~125 eV which is much above the Pr 4d threshold energy (114 eV) which confirms that there is a finite hybrization present in this system. E 0 (~125 eV) obtained for PrGe matches well with the reported value of the E 0 for thick Pr films30 and high T C superconductor Y1−x Pr x Ba2Cu3O7−δ 31.

The signature of hybridization between the 4f states and the conduction electrons is well known to give rise to features in the core level spectrum and is studied in detail in other rare-earth based systems27, 32. Pr 3d core level spectrum is shown in Fig. 2(c) where SO splitting of 20.1 eV has been obtained between the Pr 3d 5/2 and 3d 3/2 peaks. Extra features marked as  f  3 and m in Fig. 2(c) have been observed for both the Pr 3d 5/2 and 3d 3/2 peaks. The asymmetric feature m arises due to the multiplet electronic states and has also been seen in other Pr based systems33. The main peak  f  2 is associated with the poorly screened 3d 9 f2 states while the other feature marked as  f  3 arises from the 3d 9 f  3 configuration34, 35f3 feature has been attributed to 5d → 4f satellite34, 35 which also confirms the hybridization of the Pr 4f states with the conduction electrons. Since Pr 4f states carries the local moment hence the strong hybridization of the Pr 4f states with the conduction electron leads to the spin polarization which give rise to the Rashba effect in this system.

It is reported that for the light rare-earth elements, which has less than the half the maximum number of 4f electrons exhibit only weak magnetism36. This weak magnetism is associated with the antiferromagnetism and arises due to the spin canting present in the system. In this case, the magnetic moments which occupy each site of a regular lattice are assumed to be equivalent but not exactly antiparallel, leaving a net magnetization on the system. This net magnetization in the canted antiparallel arrangement gives rise to the exchange splitting. This kind of antisymmetric interaction which causes the spin canting is known as DM interaction and the microscopic mechanism is related to the spin-orbit coupling. The competition between the DM interaction and the isotropic ferromagnetic exchange interaction gives rise to the magnetism in the weak ferromagnetic system.

To explore the above mentioned possibilities in PrGe, we have performed the first principles density of states (DOS) calculations of [010] surface of PrGe within DFT using GGA method by considering the experimental lattice parameters19 and compared it with the bulk calculations as shown in Fig. 2(d–h). The SO coupling for the Pr 4f states have been included in the calculations. For the surface calculations, we have used the periodic supercell or slab model approach37. The vacuum layers of thickness of 10 Å were added to the surface to minimize interatomic interactions between periodic images of the slabs. The slab was periodically repeated in three dimensions to facilitate calculations in reciprocal space. For our calculations, we have selected Pr-terminated PrGe [010] surface (see Fig. 2) in the anti-parallel spin configuration (for Pr atoms) incorporating SO coupling. All the atoms in the surface slab were fully relaxed. Our relaxed positions of atoms indicated deviation of less than ±0.001 Å from the initial positions. We have shown the PDOS of Pr 4f and Pr 5d states of the top Pr atoms in the surface slab calculation in Fig. 2(d,e). Compared to the bulk PDOS, we find that the Pr 4f and the Pr 5d states has a larger intensity at and near E F (Fig. 2(d,e)) in the surface slab calculation. The energy position of the PDOS of all the states remain same in both the bulk and the surface slab calculation except for the Ge 4p state, which show a 0.46 eV shift towards higher energy for the surface calculation as compared to the bulk calculation (Fig. 2(g)). The Ge 4s PDOS (Fig. 2(f)) shows a slightly higher intensity in the surface calculation. The broadened PDOS of Pr 4f states obtained from the surface slab calculation (Fig. 2(h)) shows a good agreement with the experimental PDOS obtained from the difference of the on-resonance and the off-resonance spectra at 125 eV and 116 eV as shown in Fig. 2(b). There is a small shift of about 0.3 eV between the peak position of the experimental PDOS of Pr 4f states with that from the surface slab calculation of Pr 4f  PDOS. The difference between the theoretical and the experimental DOS is because the calculation has been performed for the ideal sample and the sample related effects like the complex magnetism present in this system, the actual condition of the spin polarization and antisite disorders or defects present in the system are not taken into account. At and near E F , the density of states shows a strong hybridization of the Pr 4f states with the Pr 5d states. We find that the total magnetic moment obtained for the top Pr atom in the surface slab calculation is very small about 0.009 μ B which further supports the argument that the PrGe system is indeed similar to weak ferromagnetic systems.

To further understand the behavior of the energy dispersion curves at different magnetic phases due to the DM interaction, we have shown the band structure in both k a and k c direction in Fig. 3(a–e), respectively. Interestingly, different hole-like and electron-like Rashba spin-split bands are observed in the k a and k c directions. The appearance of electron-like and hole-like bands in different direction of k-space is related to the presence of Saddle point van Hove singularity in the system38. Saddle point singularity is a clear signature of the spontaneous symmetry breaking due to the DM interaction and has been reported for the gapless topological systems with chiral magnetic structures24, 25. In presence of DM interaction39 the single particle energy for the magnetic system is: $${E}_{k,\sigma }={\textstyle \tfrac{{\hslash }^{2}}{2{m}^{\ast }}}[{({k}_{x}-\sigma {k}_{0}\sin \theta )}^{2}+{k}_{y}^{2}]-{E}_{R}\,{\sin }^{2}\,\theta -\sigma {[{({J}_{0}S)}^{2}+{\alpha }_{R}^{2}({k}_{x}^{2}{\cos }^{2}\theta +{k}_{y}^{2})]}^{1/2}$$. Here k x and k y are the momentum parallel to the surface (XY-plane) which is similar as the k c and k a direction respectively in the present scenario. σ is the carrier spin index = ±1, θ denotes the angle of the magnetization with respect to the Z-axis (perpendicular to the surface), m* is the effective mass and J 0 S = Δ represents the coupling between the magnetic impurity and the carriers where J 0 is the exchange strength and S is the spin of the magnetic impurity. α R denotes the coupling constant in the SO Hamiltonian which is described by $$\tfrac{{\hslash }^{2}{k}_{0}}{{m}^{\ast }}$$. Rashba energy E R , is described by $$\tfrac{{m}^{\ast }{\alpha }_{R}^{2}}{2{\hslash }^{2}}$$. We have simulated the energy dispersion curves considering three major conditions for the DM interaction in this system: 1) magnetization axis (M) is exactly perpendicular to the surface, in this case θ = 0, 2) M is along Z-axis but tilted in XY-plane and 3) M is parallel to the Y-axis and the direction of moment tilt away from the Y-axis in the direction perpendicular to surface, in this case θ = 90°. The detail discussion on the simulation is presented in the supplementary information.

In the experimental band structure (Fig. 1(d–m)) it is quite clear that the shift of the bands in the momentum space from the Γ point is almost constant however there is a drastic changes in the shape of the bands across the magnetic phase transition. Hence, in the simulation as shown by the solid lines in Fig. 3(a–c) we have varied the value of k 0, m*, Δ and θ¸ to understand their actual effect on the band structure. We find that the experimental observations matches very well with the third condition where M is parallel to Y-axis (supplementary information Fig. 2(c)). The important result is that only in the case of magnetization axis being parallel to Y-axis (θ = 90°) (supplementary information Fig. 3(g–i)) the Rashba SO split bands lie well below E F . Hence, the physical effect of θ is it causes a shift of the valence band maximum. From the analysis performed on the experimental band structure, we have obtain the value of k 0 ≈ 0.11 ± 0.005 Å −1 along the k c direction which is same in both PM and FM phase. The value of k 0 in PrGe [010] is about 7.3 times higher than the value of k 0 ≈ 0.015 Å −1 as reported for Gd [0001]8, 9. The electron-like states in the k c direction is lowered by an energy E R  ≈ 0.58 ± 0.002 eV w.r.t. E F . The value of m* is negative for the hole-like bands and positive for the electron-like bands. The important result obtained along the k a direction for the hole like bands is that the effective mass m* is found to increase in the FM phase (0.466 ± 0.005 m e ) and in the AFM phase (0.326 ± 0.005 m e ) than in the PM phase (0.176 ± 0.005 m e ). In the k c direction the effective mass of the electron-like states is found to be two times less as compared to the hole-like states observed in the k a direction for that particular phase. The value of α R obtained is ≈5 ± 0.02 eVÅ at 100 K. This is probably the largest value of α R obtained so far for the metallic surface states. We find that the value of α R decreases across the phase transitions from ~2.7 ± 0.02 eVÅ in near AFM phase to ~1.89 ± 0.02 eVÅ in the FM phase. The highest value of α R in the paramagnetic phase over a wide temperature range from 300 K to 60 K makes it an important material for the spintronics applications. We also report that the Rashba parameter α R in PrGe can be tuned by varying the temperature. Δ mainly causes a shift in the spin-up and the spin-down bands in the near AFM phase and in the FM phase which is quite evident in Fig. 3(b,c). Highest value of Δ ≈ 0.120 eV is obtained for the AFM phase (50 K, Fig. 3(b)) which reduces to ≈0.030 eV in the FM phase (20 K Fig. 3(c)). Spin canting with respect to the Y-axis (k a direction) can be determined from the value of α R and Δ such that the canting angle δ(k a ) = tan−1(α R (k a )/Δ). The value of canting angle is almost 90° ± 0.02° in the PM phase, 87.5° ± 0.02° in the near AFM phase and 89.1° ± 0.02° in the FM phase. Different spin canting angle at near AFM and the FM phase and finite interaction between the hole-like and the electron-like states clearly indicates that there is change in the spin-polarization of the conduction electrons at different magnetic phases. The simulated curves in Fig. 3(d,e) show poor matching with the experimental bands above the saddle point near E F the reason could be due to the coulomb interaction between the electron-like and hole-like states in the vicinity of the Fermi-level which has not been taken into account in the simulation. Broken space inversion symmetry has been reported to give rise to giant Rashba effect in the non-magnetic systems like BiTeI (α R  ~ 3.8 eVÅ)40 and Bi/Ag(111) surface alloy (α R  ~ 3.05 eVÅ)7. Giant Rashba effect in PrGe (α R  ~ 5 eVÅ) is also due to broken inversion symmetry under the influence of DM interaction.

We have performed the theoretical band structure for the surface slab calculation to further understand the behavior of the bands in both the k a and k c direction. The top Pr atom carries very small magnetic moment (0.009 μ B ) and are perpendicular to [010] surface of PrGe (Fig. 2) which is similar to the condition obtained by simulation. The effect of SO coupling (SOC) on the band structure calculation is shown in Fig. 3(f,g) respectively. The calculations done without incorporating SOC clearly does not reveal any Rashba splitting of bands which, in turn, imparts conviction to the presence of Rashba splitting observed in the calculated band structure incorporating SOC. The zoomed region around $$\bar{{\rm{\Gamma }}}$$ point in Fig. 3(h,i) clearly show the existence of saddle point singularity in this system and the orbital switching from hole-like to electron-like orbital in the $$\bar{X}^{\prime}$$-$$\bar{{\rm{\Gamma }}}$$-$$\bar{X}$$ and $$\bar{Z}^{\prime}$$-$$\bar{{\rm{\Gamma }}}$$-$$\bar{Z}$$ directions, respectively for the SOC calculations. The asymmetric bands in the $$\bar{Z}^{\prime}$$-$$\bar{{\rm{\Gamma }}}$$-$$\bar{Z}$$ direction is a clear signature of the SOC and the effect of magnetic anisotropy present in this system. Some differences between the theoretical and experimental band structure could be due to the sample related effects as well as the experimental conditions which could not be taken into account in the surface slab calculations.

For further understanding the spin structures present in this system, we have performed the magnetoresistance (MR) measurements. MR as a function of temperature is shown in Fig. 4(a,b). Negative MR has been observed in the PM phase at 60 K (Fig. 4(a)), which clearly indicates that there is a net magnetization present in this system. A large MR of 43% at 8 T field is observed in the AFM phase at 42 K. However in the FM phase 30 K the MR is more positive than the AFM phase. The reason for obtaining a large MR in the AFM phase than in FM phase could be related to the exchange splitting and the canted spin orientation which is more enhanced in the AFM phase than in the FM phase (Fig. 3(b,c)). Similar behavior in the magnetoresistance has been observed for PrGa, where a large magnetoresistance of 34% is reported at 5 T field in AFM phase41. Also it has been observed that the MR decreases and becomes more positive in the FM phase in PrGa which is attributed to the change in the lattice parameters during AFM to FM phase transition on the application of field41. Another interesting result in PrGe is that an anisotropic MR behavior w.r.t. field direction (Fig. 4(b)) is observed at all the temperatures only for the [010] crystallographic orientation (supplementary information Fig. 4). Similar anisotropic behavior in MR has been observed in the Pt/Co/Pt films42, CrO2 thin films43 and MnSi nanowires44 where it is related to the chiral magnetic structure present in these systems. The chiral magnetic structure lacks inversion symmetry and has a strong spin-orbit coupling which is mainly induced by the DM interaction. It is well known that the origin of the chiral magnetic states is related to the change of lattice structure at the crystal boundary or due to the surface contribution which generates an additional magnetic anisotropy.

DM interaction is expected to influence the lattice structure, hence we have performed temperature dependent x-ray diffraction (XRD) studies on the powder sample to probe its existence. The XRD data have been recorded at few temperatures using laboratory based (Cu K α ) source (Fig. 4(c)) and linearly polarized synchrotron source (13 KeV energy) (Fig. 4(d)). XRD patterns from lab source did not show any change in the peak profiles till the lowest temperature. This indicates no structural change across the magnetic transition and the sample retains CrB type structure with orthorhombic space group Cmcm (inset of Fig. 4(c)).

XRD patterns from the polarized synchrotron source showed some additional peaks as compared to those recorded from lab source. In Fig. 4(d) the strong peak (around 18.7°) shows signature of splitting into two peaks at 18.64° and 18.71° (shown by dotted lines in the Fig. 4(d)) observed in both heating and cooling cycles. On plotting the intensity of the 18.97° peak (peak A in Fig. 4(d)) as a function of temperature in Fig. 4(e), we find a hysteresis around the magnetic transition. Similar kind of hysteresis as a function of temperature has been observed for other peaks, which indicates the first order nature of magnetic transition that is in good agreement with our earlier work on PrGe19. DM interaction has been reported to show first order magnetic transition in MnSi45. Hence, the magnetic transition in this system are due to strong coupling between the spins and the lattice which further confirms the presence of DM interaction in this system.

The conclusions drawn from the present work are: 1) PrGe behaves like a weak ferromagnetic system in which the Pr atoms in different sublattices have antiparallel spin orientation and the evidence of strong coupling between the spins and the lattice has been obtained in the experiments. 2) Origin of giant Rashba effect on the PrGe [010] surface in the PM phase is due to the breaking of space inversion symmetry by the DM interaction. 3) DM interaction arises in this system due to the hybridization between the magnetic Pr 4f electrons with the Pr 5d conduction electrons. 4) Magnetic ordering both ferromagnetic and antiferromagnetic arises due to the competition between the DM interaction and the exchange interaction present in this system which actually causes the change in the spin-polarization of the conduction electrons. 5) In the FM and AFM phases, the effective mass of the electrons increases and the change in the spin-polarization causes a finite interaction between the hole-like and the electron-like states. Hence, we propose that the PrGe [010] surface which shows a giant Rashba effect (α R  = 5 eVÅ) in the PM phase, giant negative MR (43%) in the AFM phase and the possibility to tune the Rashba parameter by varying temperature across the magnetic transitions makes this material a very promising candidate for the AFM spintronics application.

## Methods

### Sample preparation and characterization

PrGe single crystal was grown by the Czochralski method19. The sample has been characterized by XRD, magnetization, resistivity, susceptibility and specific heat measurements.

### Angle resolved photoemission

High resolution angle resolved photoemission measurements at 10 meV energy resolution and 0.2 deg angular resolution were performed at the APE beamline of Synchrotron Elettra, Italy46. The clean surface of the PrGe single crystal was obtained by cleaving the sample in-situ in a base pressure of 9 × 10−11 mbar. The data have been recorded with a Scienta SES 2002 electron energy analyzer. The temperature dependent data are collected while heating using a liquid helium cooled cryostat. We have performed different data processing on the raw ARPES data (Fig. 1 of supplementary information) and the data presented here are processed using Curvature method47.

### Resonant photoemission

The resonant photoemission measurements  were carried out at the angle-integrated PES beamline on the Indus-1 synchrotron radiation source, India48. Experimental conditions are similar as reported in other references27, 48, 49. The sample surface was scraped in-situ using a diamond file multiple times to obtain atomically clean surface. The BE in the photoemission spectra has been determined with reference to the Fermi level of the clean gold surface that is in electrical contact with the sample at the same experimental conditions27. The intensities of the photoemission spectra were normalized to the photon flux estimated from the photo current of the post mirror at the beamline.

### Density Functional Theory

We have performed the plane-wave based first-principles calculations within the density functional theory (DFT) using the generalized gradient approximation (GGA) for exchange and correlations potential using the parametrization scheme of J. P. Perdew, K. Burke and M. Enzerhof (PBE)50. We have used the Vienna ab-initio simulation package (VASP)51, which solves the Kohn-Sham equations using a plane wave expansion for the valence electron density and wave functions. The interactions between the ions and electrons are described by the projector augmented wave (PAW)52 potentials. For our calculations, we have used the PAW potential for Ge which treats 3d4s4p states as valence and for Pr 5d4f6s (trivalent) states were treated as valence. We have performed the spin-polarized calculations for both bulk and surface structures. The expansion of electronic wave functions in plane waves was set to a kinetic energy cut-off (E cutoff ) of 350 eV for both the structures. The Brillouin-zone was sampled using Monkhorst-Pack k-point mesh53 of 8 × 8 × 8 (128 k-points in the irreducible Brillouin zone (IBZ)) and 4 × 8 × 1 (16 k-points in the IBZ) for the bulk and surface structure, respectively. Each structure, optimization was carried out with respect to a k-point mesh and E cutoff to ensure convergence of the total energy within a precision better than 1 meV/atom. The structural relaxations were performed using the conjugate gradient algorithm until the residual forces on the atom were less than 0.01 eV/Å and stresses in the equilibrium geometry were less than 5 × 10−2 GPa. The total electronic energy and density of states (DOS) calculations were performed using the tetrahedron method with Blöchl corrections52. For calculations of spin- and site-projected DOS for Pr and Ge atoms, the Wigner-Seitz radii chosen were 2.003 Å and 1.541 Å, respectively.

### Temperature dependent XRD

Low temperature XRD measurements were performed on the angle-dispersive x-ray diffraction beamline on the Indus-2 synchrotron radiation source. A high spectral resolution of about 1 eV at 10 KeV was achieved using Si(111) based double crystal monochromator54. Powder XRD of PrGe single crystal was recorded at 13 KeV excitation energy by using Image plate Mar-345 detector. The photon energy and the sample to detector distance were accurately calibrated using LaB6 NIST standard. Fit2D software was used to generate the XRD pattern from the diffraction rings obtained by Image plate data. Low-temperature XRD measurements were also done on x-ray powder diffractometer using rotating anode type x-ray source (Cu K α ) and CCR cryostat.

### Magnetoresistance

The magnetoresistance was measured along the crystallographic [010] direction while the field was applied along the easy axis of magnetization, i.e. the [001] crystallographic direction. The measurements were performed using a Quantum Design built Physical Property Measurement System (PPMS), where the resistivity is measured by means of standard four probe method.

## References

1. 1.

Rashba, E. I. Properties of semiconductors with an extremum loop.1. Cyclotron and combinational resonance in a magnetic field perpendicular to the plane of the loop. Sov. Phys. Solid State 2, 1109 (1960).

2. 2.

Zutic, I., Fabian, J. & Sarma, S. D. Spintronics: Fundamentals and applications. Rev. Mod. Phys. 76, 323 (2004).

3. 3.

Fabian, J., Matos-Abiague, A., Ertler, C., Stano, P. & Zutic, I. Semiconductor spintronics. Acta Phys. Slovaca 57, 565 (2007).

4. 4.

Nitta, J. et al. Gate control of spin-orbit interaction in an inverted In0.53Ga0.47As/In0.52Al0.48As heterostructure. Phys. Rev. Lett. 78, 1335 (1997).

5. 5.

Popovic, D. et al. High-resolution photoemission on Ag/Au (111):Spin-orbit splitting and electronic localization of the surface state. Phys. Rev. B. 72, 045419 (2005).

6. 6.

Bendounan, A. et al. Evolution of the Rashba spin-orbit-split Shockley state on Ag/Pt(111). Phys. Rev. B. 83, 195427 (2011).

7. 7.

Ast, C. R. et al. Giant Spin Splitting through Surface Alloying. Phys. Rev. Lett. 98, 186807 (2007).

8. 8.

Krupin, O. et al. Rashba effect at magnetic metal surfaces. Phys. Rev. B 71, 201403(R) (2005).

9. 9.

Krupin, O. et al. Rashba effect at the surfaces of rare-earth metals and their monoxides. New J. Phys. 11, 013035 (2009).

10. 10.

Brataas, A., Kent, A. D. & Ohno, H. Current-induced torques in magnetic materials. Nat. Mater. 11, 372 (2012).

11. 11.

Wang, C. et al. Anisotropic Magnetoresistance in Antiferromagnetic Sr2IrO4. Phys. Rev. X 4, 041034 (2014).

12. 12.

Fina, I. et al. Anisotropic magnetoresistance in an antiferromagnetic semiconductor. Nat. Commu. 5, 4671 (2014).

13. 13.

Barthem, V. M. T. S., Colin, C. V., Mayaffre, H., Julien, M.-H. & Givord, D. Revealing the properties of Mn2Au for antiferromagnetic spintronics. Nat. Commun. 4, 2892 (2014).

14. 14.

Joshi, D. A., Thamizhavel, A. & Dhar, S. K. Magnetic behavior of single-crystalline Pr5Ge3 and Tb5Ge3 compounds. Phys. Rev. B 79, 014425 (2009).

15. 15.

Janssen, Y., Dennis, K. W., Prozorov, R., Canfield, P. C. & McCallum, R. W. Exotic (anti)ferromagnetism in single crystals of Pr6Ni2Si3. Phys. Rev. B 77, 214407 (2008).

16. 16.

Kitai, T., Fujii, H., Okamoto, T. & Hashimoto, Y. Magnetic characteristics of PrCd single crystal. Solid State Commun. 52, 407 (1984).

17. 17.

Suzuki, O. et al. Magnetic properties of clathrate-like compound Pr3Pd20Ge6. J. Alloys. Comp. 408–412, 107 (2006).

18. 18.

Mulders, A. M. et al. PrRu2Si2: A giant anisotropic induced magnet with a singlet crystal-field ground state. Phys. Rev. B 56, 8752 (1997).

19. 19.

Das, P. K., Kumar, Ramesh K., Kulkarni, R., Dhar, S. K. & Thamizhavel, A. Antiferro- and ferromagnetic ordering in a PrGe single crystal. J. Phys. Condens. Matter 24, 476001 (2012).

20. 20.

Hohnke, D. & Parthe, E. AB Compounds with Se, Y and Rare Earth Metals. II. FeB and CrB Type Structures of Monosilicides and Germanides. Acta Cryst. 20, 572 (1966).

21. 21.

Schobinger-Papamentallos, P. & Buschow, K. H. J. Ferromagnetism of NdGe and PrGe studied by neutron diffraction and magnetic measurements. J. Less-Common Met. 111, 125 (1985).

22. 22.

Heide, M., Bihlmayer, G., Mavropoulos, Ph., Bringer, A. & Blügel, S. Spin Orbit Driven Physics at Surfaces. Newsletter of the Psi-K Network 78, www.psi-k.org/newsletters/News_78/Highlight_78.pdf (2006).

23. 23.

Volovik, G. E. From standard model of particle physics to room-temperature superconductivity. Phys. Scr. T164, 014014 (2015).

24. 24.

Leonov, A. O. et al. The properties of isolated chiral skyrmions in thin magnetic films. New J. Phys. 18, 065003 (2016).

25. 25.

Volovik, G. E. Flat band in topological matter: possible route to room-temperature superconductivity. J. Supercond. Nov. Magn. 26, 2887 (2013).

26. 26.

Kumigashira, H. et al. Paramagnetic-to-antiferroparamagnetic phase transition of CeSb studied by high-resolution angle-resolved photoemission. Phys. Rev. B. 56, 13654 (1997).

27. 27.

Banik, S. et al. Electronic structure of CeAg2Ge2 studied by resonant photoemission spectroscopy. Phys. Rev. B 82, 113107 (2010).

28. 28.

Banik, S. et al. Electronic structure of EuCu2Ge2 studied by resonant photoemission and x-ray absorption spectroscopy. Phys. Rev. B 86, 085134 (2012).

29. 29.

Fano, U. Effects of configuration interaction on intensities and phase shifts. Phys. Rev. 124, 1866 (1961).

30. 30.

Hwang, C., Lee, J. W., Kim, S. T., Lee, D. H. & Onellion, M. Electronic structure of Praseodymium. Solid State Commun. 103, 229 (1997).

31. 31.

Kang, J.-S. et al. Electronic structure of the quenched superconductivity materials Y1−x Pr x Ba2Cu3O7−δ . J. Less-Common Metals 148, 121 (1989).

32. 32.

Fuggle, J. C. et al. Electronic structure of Ce and its intermetallic compounds. Phys. Rev. B. 27, 7330 (1983); Fuggle, J. C., Gunnarsson, O., Sawatzky, G. A. & Schönhammer, K. Virtual-bound-state effects in core-level spectra of light rare-earth alloys. Phys. Rev. B. 37, 1103 (1988).

33. 33.

Fujimori, A. & Osterwalder, J. X-ray photoemission study of the electronic structure of praseodymium hydride. J. Phys. C: Solid State Phys. 17, 2869 (1984).

34. 34.

Feiner, I. et al. Crystal structure, magnetic properties, x-ray-photoemission-spectroscopy and specific-heat measurements on Pr2Ba04 and PrBa03. Phys. Rev. B 46, 9132 (1992).

35. 35.

Chung, J. et al. Photoemission Study of Rare-Earth Ditelluride Compounds (ReTe2: Re = La, Pr, Sm, and Gd). J. Korean Phys. Socie. 38, 744 (2001).

36. 36.

Chikazumi, S. Physics of Ferrmagnetism. Clarendon Press, Oxford (1997).

37. 37.

Arya, A. & Carter, E. A. Structure, bonding, and adhesion at the TiC(100)/Fe(110) interface from first principles. Journal of Chem. Phys. 118, 8982 (2003).

38. 38.

Campuzano, J. C. et al. Photoemission from the High Te Superconductors. J. Low Temp. Phys. 95, 245 (1994).

39. 39.

Barnes, S. E., Ieda, J. & Maekawa, S. Rashba Spin-Orbit Anisotropy and the Electric Field Control of Magnetism. Sci. Rep. 4, 4105 (2014).

40. 40.

Ishizaka, K. et al. Giant Rashba-type spin splitting in bulk BiTeI. Nat. Mater. 10, 521 (2011).

41. 41.

Chen, J., Zheng, X. Q., Dong, Q. Y., Sun, J. R. & Shen, B. G. Large magnetoresistance and metamagnetic transition in PrGa. Appl. Phys. Lett. 99, 122503 (2011).

42. 42.

Franken, J. H., Herps, M., Swagten, H. J. M. & Koopmans, B. Tunable chiral spin texture in magnetic domain-walls. Scientific Reports 4, 05248 (2014).

43. 43.

Anwar, M. S. & Aarts, J. Anomalous transport in half-metallic ferromagnetic CrO2. Phys. Rev. B 88, 085123 (2013).

44. 44.

Du, H. et al. Electrical probing of field-driven cascading quantized transitions of skyrmion cluster states in MnSi nanowires. Nat. Commu. 6, 7637 (2015).

45. 45.

Janoschek, M. et al. Fluctuation-induced first-order phase transition in Dzyaloshinskii-Moriya helimagnets. Phys. Rev. B 87, 134407 (2013).

46. 46.

Panaccione, G. et al. Advanced photoelectric effect experiment beamline at Elettra: A surface science laboratory coupled with Synchrotron Radiation. Rev. Sci. Instrum. 80, 043105 (2009).

47. 47.

Peng, Z. et al. A precise method for visualizing dispersive features in image plots. Rev. Sci. Instrum. 82, 043712 (2011).

48. 48.

Chaudhari, S. M. et al. Photoelectron spectroscopy beamline on Indus-1 synchrotron radiation source. Curr. Sci. 82, 305 (2002).

49. 49.

Pandey, P. K., Choudhary, R. J. & Phase, D. M. Anomalous temperature dependence in valence band spectra: A resonant photoemission study of layered perovskite Sr2CoO4. Appl. Phys. Lett. 104, 182409 (2014).

50. 50.

Perdew, J. P., Burke, K. & Enzerhof, M. Generalized Gradient Approximation Made Simple. Phys. Rev. Lett. 77, 3865 (1996).

51. 51.

Kresse, G. & Furthmüller, J. Efficient iterative schemes for ab initio total-energy calculations using a plane-wave basis set. Phys. Rev. B 54, 11169 (1996).

52. 52.

Blöchl, P. E. Projector augmented-wave method. Phys. Rev. B 50, 17953 (1994); Blöchl, P. E., Jepsen, O. & Andersen, O. K. Improved tetrahedron method for Brillouin-zone integrations. Phys. Rev. B 49, 16223 (1994).

53. 53.

Monkhorst, H. J. & Pack, J. D. Special points for Brillouin-zone integrations. Phys. Rev. B 13, 5188 (1979).

54. 54.

Sinha, A. K. et al. Angle Dispersive X-ray Diffraction Beamline on Indus-2 Synchrotron Radiation Source: Commissioning and First Results. J. Phys.: Conf. Ser. 425, 072017 (2013).

## Acknowledgements

The authors wish to thank Dr. P. A. Naik, Dr. Tapas Ganguli, Dr. G. S. Lodha and Dr. P. D. Gupta of RRCAT, Indore for their constant encouragement and support. Mr. Avinash Wadikar of UGC-DAE CSR, Indore is thanked for his help in the RPES experiments. Dr. Archana Sagdeo, Mr. M. N. Singh and Mr. Anuj Upadhyay of RRCAT, Indore are thanked for the low temperature XRD measurements. Ms. Ruta Kulkarni of TIFR, Mumbai is thanked for her help in performing the MR measurements. Dr. L. S. Sharath Chandra of RRCAT, Indore is thanked for helpful discussions. Dr. J. R. Osiecki of DPCB, Sweden and Dr. K. S. R. Menon of SINP, Kolkata are thanked for providing the Igor macros for the ARPES data analysis. The authors acknowledge the support provided by Department of Science and Technology, Government of India under Indo-Italian S&T POC to carry out experiments at Elettra. The authors also acknowledge the Department of Atomic Energy, Government of India for financial support.

## Author information

Authors

### Contributions

S.B., A.T. and A.B. proposed the study; S.K.D. was the project coordinator; P.K.D. and A.T. prepared the single crystals; A.B., I.V., P.K.D., N.B., J.F. and A.T. performed the ARPES experiments at Elettra; S.B. performed the RPES experiments at Indus-1; D.M.P. provided the experimental facility for the RPES experiments; S.B. and A.K.S. performed the temperature dependent XRD measurements at Indus-2; A.A. performed the theoretical DOS and band structure calculations; P.U.S. performed the low temperature XRD with Laboratory based source; ARPES and RPES data analysis has been carried out by S.B.; XRD and MR data analysis has been carried out by S.B. and P.K.D.; S.B. prepared the manuscript with the input from all the authors. All authors reviewed the manuscript.

### Corresponding author

Correspondence to Soma Banik.

## Ethics declarations

### Competing Interests

The authors declare that they have no competing interests.

Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## Rights and permissions

Reprints and Permissions

Banik, S., Das, P.K., Bendounan, A. et al. Giant Rashba effect at the topological surface of PrGe revealing antiferromagnetic spintronics. Sci Rep 7, 4120 (2017). https://doi.org/10.1038/s41598-017-02401-z

• Accepted:

• Published:

• ### Investigation of electronic structure of transition metal silicides MnSi1.75 and CoSi for enhanced thermoelectric properties

• Soma Banik

Solid State Communications (2020)

• ### Direct hybridization gap from intersite and onsite electronic interactions in CeAg2Ge2

• Soma Banik
• , A. Arya
•  & A. K. Sinha

• ### Localization of electronic states resulting from electronic topological transitions in the Mo1−xRex alloys: A photoemission study

• L. S. Sharath Chandra
• , Shyam Sundar
• , Soma Banik
• , SK. Ramjan
• , S. N. Jha
•  & S. B. Roy

Journal of Applied Physics (2020)

• ### Large positive magnetoresistance and Dzyaloshinskii–Moriya interaction in CrSi driven by Cr 3d localization

• Soma Banik
• , Shilpa Tripathi
• , R. Rawat
•  & S. N. Jha

Scientific Reports (2020)

• ### Inverse design of compounds that have simultaneously ferroelectric and Rashba cofunctionality

• Carlos Mera Acosta
• , Gustavo M. Dalpian
•  & Alex Zunger

Physical Review B (2020)

By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.